Professional Jewelry Making
A Contemporary Guide to
Traditional Jewelry Techniques
Barry Blau and Christine Dhein
George McLean and emiko oye
318 Bath Road
Brunswick, Maine 04011
© 2011 by Alan Revere. All rights reserved.
Photography by Barry Blau and Christine Dhein
Illustrations by George McLean, emiko oye, and Alan Revere
Book design: Kathleen Cunningham Design
Originally published as Professional Goldsmithing
© 1991 by Van Nostrand Reinhold
Reprints of original engravings from L‘Encyclopédie, ou
dictionaire raisonné des sciences, des arts et des métiers by
Denis Diderot. Courtesy of the Brancroft Library and the
Revere Academy of Jewelry Arts.
Printed in Hong Kong
WARNING: Some of the traditional procedures described in this
book can be harmful if not executed properly. Learn about the
hazards of all techniques and materials before using them. Wear
protective goggles and use proper safety measures. When in doubt,
consult an expert.
All rights reserved. No part of this book may be reprinted or utilized
in any form or by any electronic, mechanical or other means, now
known or hereafter invented, including photo-copying, recording,
scanning, or by any information storage or retrieval system without
permission in writing from the publisher.
This book as well as a complete listing of instructional
opportunities for jewelers is available from:
Revere Academy of Jewelry Arts
760 Market Street, Suite 900
San Francisco, California 94102
(415) 391-4179 or fax (415) 391-7570
Many generous people have helped in the preparation of
this book. During my practice and education I have met
and shared information with countless craftspeople and
other experts, each offering a unique point of view based
on their own personal experiences. In 1972, in search of
training that I could not find in the United States, I traveled
to Pforzheim, Germany, a town known throughout
the world as the “Gold City.” Pforzheim is located in the
Black Forest region, and for nearly two hundred years it
has served as a major international center of goldsmithing
and jewelry manufacturing. For two years I had the
good fortune to study at Pforzheim’s world-renowned
Fachhochshule für Gestaltung, formerly the Kunst und
Werkschule, with students from jewelry communities
around the world. Indeed, the school has trained leaders
in the jewelry industry for well over a hundred years.
Jewelry historian Ralph Turner noted that the Pforzheim
school “has probably produced more creative jewellers
than any equivalent anywhere else in the world.” 1
Professor Reinhold Bothner was most responsible for my
training as a goldsmith. At the time that I worked with him,
he was the senior master goldsmith in Pforzheim, having
spent half a century creating treasures. I studied design
with Professor Reinhold Reiling, a master goldsmith and
internationally acclaimed jewelry designer. Professors Föll
and Zeiss trained me in the skills of hand engraving and
stonesetting, respectively. In addition to my classes and
studio work, I was employed in several workshops, including
that of Klaus Ullrich, a renowned designer, master
goldsmith, and master silversmith. It was while working for
Professor Ullrich that I learned how to use precious metals.
Many other dedicated craftspeople helped me gather the
information presented in this book. We all share a love of
fine metal work and together are carrying our craft into
the next millenium. Some are senior members of the
jewelry community, and some are newcomers whose
enthusiasm has helped keep the torch lit. Among these
fine craftspeople are George McLean, Evert DeGraeve,
Edward Friedman, Michael Good, Yas Tanaka, Jon T.
Dixon, Karen Sprague, Paul Christiansen, Harold
O’Connor, Steven Kretchmer, Jaime Pelissier, Doug
Zaruba, Frank Trozzo, George Sawyer, Joannie Mar,
Wellington Dong, Julie Harrington, Holly Beye, Emmy
McKenzie, Neal Pollack, Irene Hogan, Irving Gold,
Enrique Lopéz Larrea, David Clarkson, Keith Bartel,
Abrasha, Michael Smorra, and Gregory Steerman. In
addition, I wish to thank the many students at the Revere
Academy of Jewelry Arts who helped me prepare the
material for this book including: John Sliwa, Bruce Morrison,
Catherine Glew, Jay Vullings, Keith Saslaw, Eric Baltzley,
Vinnie DiPadova, Terry Cook, Jeff Gray, and Kristin Baker.
Two modern masters, Tim McCreight and Charles Lewton-
Brain, contributed significantly to this project through their
service as technical editors. I would like to thank George
Holmes, the editor of Jewelers’ Circular-Keystone where
much of this material first appeared, as well as Lilly
Kaufman of Van Nostrand Reinhold for her support; Anna
M. Miller for putting me in touch with VNR; and jewelry
writer and critic Ettagale Blauer for her encouragement.
I would like to thank Bill Nigreen and Max Yasgur who
colluded to save me from law school, as well as Andrew
Wilner who showed me that crafts could be a way of life. I
acknowledge Carolyn Chaikin Rosenberg who introduced
me to art and craftsmanship at an early age. In addition to
the photographs, Barry Blau has given this project many
years of his tireless perfectionism and humor, both in the
original and now revised edition.
The reworking of Professional Goldsmithing into Professional
Jewelry Making was possible thanks to the tireless
hours by my assistant, Christine Dhein, and book designer
Kathleen Cunningham. Also thanks to Yas Tanaka and
James Binnion for technical assistance, to emiko oye for
her work on the illustrations, and to Robert Graham for his
eye in proofing the text.
Finally, I wish to thank Sherli and my father George for
their support, patience, and encouragement during my
journey, as well as my children Dustin and Alexis, who
inspired me to prepare this material for future generations.
1 Ralph Turner, Contemporary Jewelry (New York: Van Nostrand Rein-
hold, 1976), p. 46.
Part 1 Getting Started
Part 2 Basic Projects
Curb & Cable Chain
Precious Metals 2
General Procedures 15
Alloying & Ingots 42
Part 3 Advanced Projects
Pierced Bezel Ring
Rolling Wire 48
Annealing Wire 56
Drawing Wire 57
Using a Vernier Caliper 58
Sharpening a Drill Bit 67
Throughout this book you will find several dozen Technique
Boxes like the one shown here. These present highlighted
information on specific techniques in condensed form that is
easy to locate. To revisit a particular box, use the index below.
Rolling Wire Flat 73
Filing Flat 77
Step Rolling 104
Filing the Inside of a Ring 107
Using a Sanding Stick 108
Sanding the Inside of a Ring 109
Pick Soldering 120
Filing Outside a Curved Plane 125
Using Binding Wire 128
Linear Forging 134
Making Tubing 140
Tension Soldering Tubing 142
Dividers to Lay Out a Circle 161
Dapping a Hemisphere 176
Annealing Platinum 279
Welding Platinum 287
In the early 1700s a French philosopher, art critic, and
writer named Denis Diderot began the monumental work
of creating the largest encyclopedia of his time,
L’Encyclopédie, ou dictionnaire raisonné des sciences, des
arts et des métiers (The Encyclopedia or Rational Dictionary
of the Sciences and Trades). Through twenty-eight volumes
of highly detailed engravings, Diderot documented the
technology of pre-industrial Europe. The original 1751 edition,
which was later revised, covered hundreds of subjects
in great detail, from the art of gardening to the art of war,
from belt making to barrel making, and from blacksmithing
Nearly three centuries have passed since Diderot’s encyclopedia
first appeared, and in that time, most of the trades he
described and illustrated have either disappeared or have
been mechanized by modern technology. Interestingly
enough however, the art of jewelry making has remained
virtually unchanged. Jewelry makers today still fabricate
rings and bracelets in much the same way as did the artisans
of Diderot’s time, and moreover, the tools they use
have remained nearly identical to those that Diderot documented.
And despite the passage of nearly three centuries,
the finest jewelry is still made the old fashioned way, by
This book follows the spirit of Denis Diderot, documenting
the practice of making jewelry using precision photography
along with detailed technical instructions. The material in
this book was compiled in the workshop of the Revere
Academy of Jewelry Arts in San Francisco, California, and
is based on classical goldsmithing education as handed
down for generations. It describes a series of practical projects
including rings, chains, bracelets, earrings, and
clasps. The work was executed by Alan Revere, a modern
master jeweler, and is presented in a graduated format.
Each project has been successfully completed by student
jewelers following the instructions presented in this book.
Professional Jewelry Making is a revised and expanded
version of Professional Goldsmithing, by Alan Revere,
originally published in 1991. This edition includes
larger photographs that have been refined and corrected
to show the greatest level of detail. Professional Jewelry
Making includes five new chapters as well as a totally
new look and layout.
The projects in this book are generally arranged in order
of difficulty; that is, the first few are the easiest and they
become more challenging as the book progresses. Later
projects may include techniques introduced earlier.
Because skills are presented as they are needed and some
procedures are used in several projects, we presume that
the reader will be familiar with those techniques already
discussed in earlier chapters. In many cases, several different
techniques can be used to achieve the same results,
and so different solutions to the same type of problem are
demonstrated in different projects.
Before embarking on a project, it is best to read through
the procedures and study the illustrations. Try to understand
and visualize what is happening. Try to imagine how
the metal is being transformed, how the tools affect it, and
what it should look like when completed. While you are
making a new piece, keep a journal in which you can take
notes and make sketches. You could even place the finished
piece of jewelry on a copy machine and paste the
image into your journal.
Above all, enjoy yourself. The purpose of undertaking
these projects is to build and improve your skills. Take the
time required, without distraction, to do your best. While
the purpose is to challenge yourself and learn new skills, do
not attempt a project that is too far beyond your current
level. It is more rewarding to complete a simpler project
well than to struggle and meet frustration at every turn in a
more advanced one.
This book is intended for anyone interested in making jewelry
and doing fine metal work. For beginners it provides a
graduated course of study in the art of making jewelry, with
an emphasis on hand skills. For experienced jewelry bench
workers, the projects provide a chance to increase technical
versatility. And for the jewelry collector, historian, and
merchant, this book demystifies one of humankind’s oldest
and most refined art forms.
The projects are presented clearly and concisely, with stepby-step
instructions for replication in a small jewelry workshop,
with photographs and text to show how to hold each
tool and fabricate the components of each project. Instructions
reveal trade secrets and tricks that are rarely taught in
schools and seldom shared in today’s jewelry industry.
An old master once said, “The art of
jewelry making is really very simple
and can be summarized by ten techniques.
However,” he said with a smile,
“there are ten thousand tricks.”
Chapter Precious Title Metals
Throughout history, precious metals have been
highly valued and sought after. Precious metals are
extremely durable because they are highly resistant
to attack from the environment, most acids, and tarnish.
The title noble metals refers to the high value and enduring
quality that sets these metals apart from all other elements
found in nature.
Gold was probably the first metal discovered, and it has been
used to fashion objects of special value and adornment for
thousands of years. Gold is the king of metals in several
regards. It is the only yellow metal and it is more visually
striking and workable than all others. Silver has also been
widely used and appreciated since antiquity for its high
degree of workability and for its white lustrous appearance.
Platinum, although found in pre-Columbian artifacts, was
not significant in jewelry until the nineteenth century.
There is a total of eight elements under the collective grouping
of precious metals; they are gold, silver, and platinum,
and the five other metals in the platinum family: iridium,
osmium, palladium, rhodium, and ruthenium (Table 1.1).
Number Jewelry uses
Gold au 79 Usually alloyed with
other metals for
Silver ag 47 Usually alloyed with
7.5 percent copper
to make sterling
Platinum Pt 78 Usually alloyed with
other metals for
Iridium Ir 77 Traditionally added
to platinum to
Palladium Pd 46 Used to make setter’s
white gold. contemporary
use on its own
rhodium rh 45 electroplated over
white metals for
ruthenium ru 44 Sometimes added to
platium and gold for
Osmium Os 76 Too hard for jewelry
Table 1.1 The precious metals.
Their durability, appearance, and malleability make all of
the precious metals (except osmium) ideal for use in jewelry.
A metal is an element characterized by a distinctive luster,
malleability, ductility, and thermal and electrical conductivity,
or is an alloy of such metals. In turn, an alloy is a
mixture or combination formed by the fusion of two or
more metals. Pure metals are elements and cannot be
separated or purified further. Of the 79 metals among the
103 naturally occurring elements, only 4—gold, silver,
platinum, and copper—are found in metallic form in
nature. Native metals, as these are called, are rarely pure
but are usually found in natural alloys with other metals.
Native gold, for instance, is generally combined with varying
proportions of silver; when it contains approximately
50 percent silver, it is called electrum. The six platinum
metals are found together in nature and share similar characteristics,
in fact, the six were not completely distinguished
until the nineteenth century.
chapter 1 | Precious Metals 3
Gold has been used in jewelry for over seven thousand
years! The beauty of pure gold is incomparable. As the only
yellow metal, its rich, deep yellow color and its substantial
weight are universally appealing. Ancient people associated
gold with the sun and gold has always stood for wealth and
power. Throughout the ages, most of the gold that has been
mined has been used to make articles of jewelry and ornamentation.
Even today, approximately 56 percent of the
world’s output of gold is used to make jewelry. Another 13
percent is consumed by electronics, industrial, and dental
uses, and 31 percent winds up as gold coins, bars, and other
investments (World Gold Council 2009). Gold has often
been the standard on which paper currency is based. Until
1939, the paper money of the United States was backed by
gold, meaning that upon demand at a bank anyone could
redeem gold for their paper money.
Gold is the most malleable (i.e., “softest”) of all metals,
which means that it requires the least effort to bend and
shape. It is also the most ductile, making it easiest of all
metals to draw into a long wire without breaking. In fact,
1 ounce of gold can be drawn into a fine thread several
miles long. Pure, or fine, gold is exceptionally well-suited
4 Professional Jewelry Making
to chasing and forging, but like pure silver and pure platinum,
it is generally considered too soft for jewelry due to its
vulnerability to scratching, denting, and wear. Some Asian
(mainly Chinese) jewelry is made with pure gold, but in
the West, pure gold is rarely used in jewelry, except in certain
cases. For instance, fine gold and fine silver are used
in enameling, and occasionally a bezel is made of pure
metal to facilitate the setting of very fragile gemstones.
Most often though, pure gold is alloyed with copper and
silver in varying proportions to produce the wide range of
karat gold alloys used in jewelry (Illustration 1.1). The proportions
of these three metals determine the color and
working characteristics of the alloy.
Gold and other precious metals are weighed and traded
internationally in troy ounces. In this ancient system, 1 troy
ounce equals 20 pennyweight (dwt), each of which contains
24 grains. In the metric system, 1 troy ounce equals
The purity or fineness of gold alloys is based on the propor-
tion of pure gold to other metals. The measure of gold’s
purity is expressed as its karat, abbreviated K, Kt, k, or kt in
the United States. In Great Britain the spelling is carat,
abbreviated c or ct. The term carat also refers to a completely
Illustration 1.1 Diagram of the au–ag–cu ternary system.
separate system used to weigh precious gems. One carat
equals 0.2 grams. This usage has ancient roots, derived from
the consistent weight of a carob seed.
In the karat system, gold’s purity is measured in twenty-four
parts, and so fine gold (100 percent pure) contains twentyfour/twenty-fourths
gold, which is stated as 24k. An alloy
that contains 75 percent, or eighteen/twenty-fourths gold is
18k. The fineness of precious metals can also be expressed
in parts per thousand, which is the international system
used in most other countries, making pure gold 1000 fine,
and 18k equal to 750 fine. Pure gold thus can be stamped
either 24k or 1000. Gold suppliers offer a wide variety of
alloys, or karat golds, to meet specific needs such as casting,
fabrication, or pinstems for brooches (Table 1.2).
Eighteen-karat gold is the international standard for the
finest gold jewelry. This alloy is 75 percent pure and highly
workable. It is composed of 18 parts gold by weight and
6 parts other metals, making it a nearly perfect compromise
between pure gold’s rich yellow color and feel, and the
increased hardness and durability made possible through
alloying. The exact composition and proportion of the
non-gold components depends on the color and working
characteristics that are sought (see Physical and Mechanical
Properties of 18k Gold Alloys in the Appendix).
Silver and copper are the primary metals added to make
18k alloys. When there is a greater proportion of silver, the
result is a softer gold alloy with a greenish tint. Red-gold
alloys contain a greater proportion of copper, which raises
the hardness. An 18k alloy with an equal amount of silver
and copper is a deep yellow color. It is very workable and
ideal for most jewelry applications. Small amounts of zinc
are sometimes added to karat golds in order to lower the
In England, 18k gold became legal for jewelry during the
fifteenth century, and it has been used for jewelry ever
since. In the United States, 18k gold is used for the finest
gold jewelry, with the majority of commercial jewelry
being produced in 14k gold.
Parts by Weight
Karat Gold Other Metals Fineness Uses
24k 24 0 1.000 Bullion, some asian jewelry.
23k 23 1 .958
22k 22 2 .916 Highest standard for gold jewelry in Britain and Japan.
21.6k 21.6 2.4 .900 coinage
21k 21 3 .875
20k 20 4 .833
19k 19 5 .792
18k 18 6 .750 International standard for better gold jewelry: Japan, United States,
Germany, and Britain. Lowest legal standard permitted in france and Italy.
17k 17 7 .708
16k 16 8 .666
15k 15 9 .635
14k 14 10 .585 Most common alloy for gold jewelry in the United States , Germany,
and Japan. Lowest legal standard permitted for gold jewelry in austria,
Denmark, and Norway.
13k 13 11 .542
12k 12 12 .500
11k 11 13 .458
10k 10 14 .417 Lowest legal standard permitted for gold jewelry in the United States
9k 9 15 .375 Lowest legal standard permitted for gold jewelry in Britain, canada,
8k 8 16 .333 Lowest legal standard permitted for gold jewelry in Germany.
Table 1.2 Gold karat, fineness, and uses.
In the United States, most gold jewelry is 14k, or 14/24, gold.
Fourteen karat gold is 58.333 percent pure gold. Convention
has converted this number to the more manageable and
slightly finer 58½ percent gold, which can also be expressed
as .585, or 585/1000 pure. This quality is stamped 14k in
the United States, and often 585 in Europe. The remaining
41½ percent is usually composed of silver and copper.
Fourteen karat gold is harder than 18k and more durable
for jewelry use, although it is paler in color. The more
copper there is in 14k alloys, the redder the color will be (see
Physical and Mechanical Properties of 14k Gold Alloys in the
Appendix). Likewise, the greater the proportion of silver is in
the alloys, the greener the color and generally the softer the
chapter 1 | Precious Metals 5
material will be. Rings, chains, and settings made of
14k gold will outlast similar items made of 18k, because
of the increased hardness. Most 14k gold alloys need to
be annealed more frequently than do 18k alloys, and most
14k gold alloys are less resistant to tarnish than higher karat
alloys. In addition, 14k gold is considerably less expensive
than 18k gold because it contains approximately 20 percent
less pure gold. It is also less dense, further lowering the cost
compared to that of 18k gold.
White gold alloys were developed in the twentieth century
as a substitute for platinum. White gold can be produced
in several finenesses, including 14k and 18k. Two types of
6 Professional Jewelry Making
white gold are most often used in jewelry manufacture:
alloys that contain nickel and alloys that use palladium.
Nickel white golds employ nickel as the bleaching agent,
and produces the least expensive white-gold alloy. The
addition of nickel hardens gold alloys, making them more
durable and able to take a higher polish. Its hardness makes
nickel white gold less desirable for forging, forming, and
especially for bright-cut or bead setting.
Palladium white-gold alloys are called setter’s gold. They
are grayer in color and better suited for gem setting, especially
bright-cut or bead setting. Palladium white-gold
alloys are more costly than nickel white-gold alloys,
because palladium itself is a precious metal. Other metals
that can be found in white-gold alloys include platinum,
silver, copper, zinc, and manganese.
Silver is an important precious metal and is used in jewelry
all over the world. It has been prized throughout history
for its unique whiteness, high degree of reflectivity and
excellent working characteristics. As a pure metal, silver
is second only to gold in malleability and in ductility. Aside
from its use as a component in most gold alloys, silver is
the principal component of sterling silver. Pure silver is
generally considered too soft for use in jewelry and other
objects and is usually alloyed into the universally standard
sterling quality. Sterling silver contains 92½ percent silver
and 7½ percent copper; it is easy to work yet durable
enough to stand up to extended wear.
fIrescAle on sterlIng sIlVer
After silver alloys are heated, a characteristic stain frequently
appears on the surface. This stain is called firescale and is a
result of the oxygen combining with copper, where it forms a
subsurface copper oxide.
The risk of firescale is increased by exposing the metal to
high temperatures for extended periods during both annealing
and soldering. Firescale is not immediatly noticeable
because it is hidden by the effects of a process called depletion
plating. During the pickling process, surface oxidation
and nonprecious metals in the alloy are removed, raising the
fine metal content on the surface, thereby concealing the
stain. Firescale then usually appears during sanding and polishing,
which breaks through the surface layer of metal,
revealing the purplish stain below.
The two approaches to dealing with firescale are prevention
and remedy. If the metal is sealed from oxygen, the
chances of firescale occurring are diminished. This can be
accomplished by heating the metal in a controlled atmosphere
without free oxygen to combine with the copper in
the silver alloy. Unfortunately it is not possible to control
the atmosphere in the ordinary jewelry workshop, and so
the jeweler’s most effective firescale preventative is to coat
the metal with a thin layer of flux before heating it. When
it is heated, the flux glazes the surface, like a clear enamel,
and blocks the penetration of oxygen. Several formulas, all
of which include borax, are at least partially effective for
preventing firescale. The most common formula for fire
coat protection is an equal amount of powdered boric acid
mixed with alcohol. Before being heated, the metal can be
immersed in the mixture or it can be painted with the solution.
Then, when the alcohol is ignited, the boric acid is
released to coat the surface. Use caution when doing this,
as it can start a fire.
Prip’s flux , another solution that is applied in a similar
manner for this purpose has the benefit of not being flammable.
Note, however, that no formula works all of the
time. Thus when using with silver, it is best to minimize its
exposure by heating it quickly. This prevents prolonged
exposure to oxidation and reduces the effects of firescale.
After firescale has appeared, it can be removed mechanically,
chemically, or electrolyticly. Mechanical methods
such as filing, sanding, and grinding remove the surface
layer containing firescale, but this is often not practical
because it is very time-consuming and distorts the dimensions
and surface of the work. Chemical methods used to
dissolve the discolored oxidation also usually result in a
finely textured surface. The electrolytical method for
removing the surface is called electrostripping and is virtually
the reverse of electroplating. In electrostripping, the
surface metal is pulled off and deposited on the cathode in
an electrolytic bath. But, this too is not a perfect remedy, as
it also leaves the surface with a characteristic texture. An
additional treatment of firescaled surfaces is to electroplate
over the area. Unfortunately this is merely a cosmetic
emedy that will only temporarily mask the firescale. The
best approach is to prevent the buildup of firescale by using
an anti-firescale “fire coat” and reducing the metal’s exposure
time during heating.
tHe PlAtInUm fAmIlY
Platinum has been used since the sixteenth century, when
it was discovered in South America. Initially it was associated
with silver (plata in Spanish). Platinum is the most
common and most widely used of the six metals in its family.
Three of the metals—rhodium, ruthenium, and palladium—are
light, having a specific gravity around 12. The
other three—osmium, iridium, and platinum—are heavy,
with a specific gravity nearly twice as high, around 21 or 22
(see Table 1.4). Grouped in another way, three of the metals—
palladium, platinum, and rhodium—have even higher
melting temperatures, between 1550 and 1970°C. The other
three—ruthenium, iridium, and osmium—have very high
melting temperatures, over 2200°C (see Table 1.5). All of
these metals are highly resistant to corrosion, and aside from
osmium, which has no jewelry application, they are used by
jewelers. Osmium, even annealed, is so hard that it is virtually
unworkable and so it is used where extreme durability is
required, such as for the tips of fountain pen nibs.
Platinum is used in jewelry because of its high degree of
workability and its white tarnish-free color. Most commonly,
platinum is alloyed with iridium, palladium, or ruthenium to
Density Hardness (Vickers)
Metal (g/cm3) annealed cold worked
Gold 19.32 20 58
Silver 10.49 22 100
Platinum 21.45 37 108
Palladium 12.02 37 106
rhodium 12.41 123 260
Iridium 22.65 220
Osmium 22.61 400
ruthenium 12.45 220 360/750
Source: Grimwade 2009.
Table 1.4 Density and hardness values for the precious
metals at 20ºc.
increase its hardness. Platinum and its jewelry alloys behave
similarly to gold in such areas as sawing, filing, drilling, rolling,
drawing, forming, and forging. Noteworthy differences
occur when soldering and polishing platinum alloys. During
soldering, the melting temperature of the solders is so high
that the metal is heated to a cherry red (which requires the
use of very dark welder’s goggles).
It is good practice to work platinum in a clean station.
Many jewelers have a dedicated workbench and soldering
station just for platinum work. If you cannot have a dedicated
workstation for this purpose, you should do a thorough
cleaning of your workbench and soldering station
because residues of other metals can contaminate the platinum
work. For example, it is important to clean all files so
that metal stuck in the teeth of your files will not be
embedded in the platinum and contaminate the piece.
With the advent of new technologies in the jewelry field, platinum
work has become easier, or at least less time consuming.
There are new filing tools (Valtitan files are excellent for platinum
work); new sanding media (micron graded sheets, film,
and strips); new polishing technologies (rubber, silicone, and
ceramic polishing wheels); new platinum polishing compounds,
and radial bristle disks; and new soldering technologies
as well (platinum soldering goggles, tungsten soldering
picks, and tungsten or ceramic-tipped tweezers for soldering).
These new technologies have made it easier for jewelers to
work in platinum with confidence.
Metal ºC ºF
Silver 961 1762
Gold 1064 1947
Palladium 1772 3222
Platinum 1552 2826
rhodium 1966 3571
ruthenium 2250 4082
Iridium 2410 4370
Osmium 3045 5513
Source: adapted from Grimwade 2009.
chapter 1 | Precious Metals 7
Table 1.5 Melting points of precious metals.
8 Professional Jewelry Making
workIng wItH PlAtInUm
In most ways platinum behaves in a manner similar to gold
and silver. Alloys of all three metals are highly malleable,
ductile, and workable. Platinum and its jewelry alloys are
filed, sawed, drilled, rolled, drawn and formed in an identical
manner to gold and silver. Because of its hardness, however,
platinum requires greater force during most mechanical
processes and several extra steps when finishing.
A major difference is encountered when soldering platinum.
Aside from its hardness, platinum is extremely resistant to
oxidation and attack by the environment. It has a very high
temperature range for soldering and is a very poor conductor
of heat. For theses reasons, procedures for soldering platinum
are quite different from working with karat golds.
Platinum items to be joined must fit together perfectly before
soldering, even to a higher standard than for gold. When polishing
platinum, components must be sanded to a higher
degree than for gold. It is helpful to prepolish all platinum
components prior to assembly, a procedure that is frequently
carried out in gold jewelry fabrication as well.
PlAtInUm AlloYs for JewelrY
Pure platinum, like pure gold and silver, is too soft for use
as jewelry. It is generally alloyed with other metals to
increase its hardness. The most common platinum alloys
are composed of 5 to 10 percent iridium, as well as other
alloys that include 5 percent ruthenium or 7.5 percent palladium.
Its high density and cost make platinum jewelry
considerably more expensive than an identical item in
karat gold. Offsetting this increased cost is the fact that platinum’s
durability permits components to be thinner and
more delicate than those possible in gold fabrication.
Due to platinum’s very high annealing, melting, and sol-
dering temperatures, it is absolutely essential to wear dark
welding goggles with a #5 filter to protect the eyes from the
blinding white light emitted. Even darker filters can be
used when melting platinum. An alternative to wearing
goggles is to hang a rectangular filter of the appropriate
obscurity in front of the work area during heating. Warning:
Even the darkest sunglasses are not acceptable as protection
when heating platinum.
Because of platinum’s high temperatures and resistance to
heat conduction, a bright oxidizing flame is used when soldering,
welding, and melting platinum. Any oxygen-fuel
system will work for soldering platinum: hydrogen -oxygen
is ideal and oxygen-natural gas, and oxygen-propane work
well. Oxygen-acetylene is the least desirable. When heating—during
melting, soldering, or fusing—try to work
quickly, minimizing the metal’s exposure to heat.
Because of its very low thermal conductivity, platinum can
be welded or fused. The advantages of welding are that an
additional level is added above the usual grades of solder
while creating a joint that is clean and invisible. To close a
ring shank by welding, roll out a small piece of the same
platinum alloy to about 0.2 mm thick. Cut a small flat snippet
slightly larger than the cross section of the ring. Use
tension to hold it in place between the two sides of the
shank. Heat the snippet directly, unlike working with gold,
where heat must reach solder by conduction from warmer
nearby areas. Heat intensely until the metal flows forming
in an invisible joint of solid metal. File to clean up excess
metal. A second level of welding can be carried out using
pure platinum (which has a slightly lower melting temperature
than a 10 percent iridium alloy) as the filler material.
After welding, many levels of solder are available for use
with platinum. These begin at about 1700°C and drop in
approximately 100° intervals down to as low as 900°C.
Therefore complex pieces can be assembled in several soldering
stages with decreasing melting temperatures. In
addition, due again to the low heat transfer of platinum, it
is possible to use the same level of solder very close to prior
seams without disturbing them.
In all soldering operations involving platinum, extra care
should be taken to make sure that components fit together
perfectly. Platinum solder will not fill in gaps. Avoid using
ordinary steel or iron tools such as tweezers, soldering
picks, and binding wire that will contaminate the metal if
heated together. Tungsten carbide works well for a soldering
pick and soldering tweezers.
Platinum does not oxidize or tarnish at all, and therefore
does not require flux. Neither fire coat nor pickling is
Whenever possible, hold the work in the air, not on a soldering
pad or charcoal block. The bottom of an alumina
crucible works well if a flat soldering surface is needed.
Rings and other small objects should be held in a thirdhand
(mounted soldering tweezers) or other insulated
cross-locking tweezers. Tweezers should hold the work at a
point distant from the area to be heated, to prevent contamination.
Either fine-nose tweezers or a wet brush can be
used to pick up and transport the solder to its destination.
Use many very small pieces of solder placed carefully along
the seam, rather than a few large pieces.
Because the low thermal conductivity prevents the spread
of heat over a large area, heat is directed to only a small
area. There is no need to preheat or warm nearby areas.
When soldering small items such as ring shanks, use a
small, very hot flame directed at the seam. Platinum solder
cannot be pulled along a seam as is possible when working
with gold. Because of the slow heat transfer, the back of a
platinum ring can usually be soldered without fear of overheating
a gem set on top of the ring. Heat the solder
directly until it flows, a distinct difference from gold procedure.
When joining platinum to gold, use the appropriate
Charcoal burns away quickly at the high temperatures
needed for platinum. For this reason, use an alumina or
ceramic soldering pad intended for this purpose.
Platinum should be annealed when rolled or drawn to twothirds
of its original thickness. Platinum must be absolutely
clean prior to heating. The metal should be placed on a
clean ceramic block used only for this purpose. Use a
bright oxidizing flame to heat small objects such as rings,
and hold them at a bright orange color for thirty seconds.
Large items require longer times for annealing. After heating,
the metal can be air cooled or quenched in water.
When recycling platinum scrap, only the very cleanest,
solder-free metal can be melted without refining because
platinum is easily contaminated by trace amounts of other
metals. Melt small quantities at a time, and weld them
together if larger pieces are needed. Do not attempt to
melt large ingots. Place the metal in an alumina crucible,
and heat with a very hot oxidizing flame until it melts and
congeals into a button. Allow the metal to air cool or
quench it in water after the red glow is gone. The round
button can be hammered, rolled, sheared, and drawn to
the size and shape desired.
The strength and permanent brilliant white luster of polished
platinum make platinum the perfect choice for areas
that are to be pavé set with diamonds. Again its hardness
enables the metal to be extremely thin while retaining its
strength. Prior to setting, the metal should be annealed
evenly to avoid hard and soft spots. Normal stone setting
burs can be used effectively on platinum. Platinum
responds well to engraving.
Platinum is more difficult to polish than gold because of its
hardness and high density. Since the metal does not oxidize
during soldering, pieces should be prepolished whenever
possible before assembly. This is advantageous because
small pieces are often easier to polish before they are
joined to others. Platinum must be finished with more steps
and more exacting craftsmanship than required for gold or
silver. After rough filing or sawing, use fine #4 or #6 files to
achieve a finer finish. Sand with a sequence of abrasive
papers starting with 240 and going through 400 and 600
paper. Buff with bobbing compound and then tripoli.
Polish with a hard platinum rouge such as white or yellow.
chapter 1 | Precious Metals 9
In Egypt as early as 2000 B.C., items of gold were tested and
marked to indicate their purity. The term hallmarking
derives from Goldsmith’s Hall in London, which has overseen
the marking of gold in England since 1300 ce. Most
countries base their system of hallmarking at least in part on
10 Professional Jewelry Making
the English system. Each country sets its own standards for
gold alloys and is responsible for enforcing them. Underkarating
is the fraudulent stamping of precious metals, indicating
a higher quality than an alloy really is. Underkarating
is both a moral and a criminal offense punishable under the
law. In fact, until 1815, hallmarking violations in England
could result in a sentence of death.
Four systems of enforcement are currently used around
In England and France, jewelers must submit every item
manufactured of precious metal to a regional office for testing
and stamping. Items that do not meet the standards for which
they are submitted may be destroyed by the testing facility.
VolUntArY HAllmArkIng wItH
PerIodIc goVernment AUdIts
In countries such as the United States, hallmarking and
quality standards for items made of precious metals are also
regulated by law. Individual makers are accountable for
adhering to them, yet they are rarely checked by government
audits. In the United States, The National Gold and
Silver Marking Act dictates the standards and requirements
for marking precious metals. Originally enacted in 1906
and revised several times since, this law requires the maker
and seller of precious metal objects to indicate the quality
and maker’s (or another’s) registered trademark, indicating
who is responsible for ensuring that quality. The maker’s
mark must be the same size as the quality mark, and be
placed as close as possible to it. As of October 1, 1981, gold
items without solder that are imported, exported, or transported
through the United States must be of a fineness not
lower than 3/1000ths parts of that indicated. Those items
that contain solder have a greater tolerance and may be
7/1000ths lower than the indicated quality. Items that combine
two identifiable metals should bear the quality mark
of both, for example, “14k and Sterling.”
The Federal Trade Commission has published a booklet
entitled Guides for the Jewelry Industry that defines jewelryrelated
terms and describes deceptive or misleading practices
and other misrepresentations of products and processes
involved in jewelry manufacture and sale. Violations
of these laws can result in fines or imprisonment or both.
Voluntary hallmarking leaves the quality and hallmarking
up to the manufacturer without governmental supervision.
Some countries, such as Germany, do not require an offi-
cial assay. Instead, quality standards and hallmarking are
supervised by credentialed master goldsmiths whose
licenses entitle them to mark items of precious metals.
Items of gold jewelry for import into many countries are
tested as they pass through customs. A small sample, often
scraped at a solder seam, is tested for quality. In order to be
imported and sold in that country, the quality must be
equal or superior to that indicated on the hallmark, or else
the items can be refused entry.
of PrecIoUs metAls
The physical properties of precious metals come into play
when they are worked. Each alloy has a characteristic
response to the forces exerted on it during forming, forging,
bending, rolling, and drawing. Alloys are selected for specific
applications because of these properties.
A metal’s hardness refers to its resistance to denting. The
hardness of metals is measured scientifically by pressing a
very hard object of a known size with a known force into
samples of different metals and measuring the results. Factors
affecting the hardness of metals include the composition
of the alloy and the degree to which it has been
worked. The three different testing and measuring systems
for hardness are Brinnel (HB), Rockwell (HR) and Vickers
(HV). (Values from one system can be compared to values
from a different system using an appropriate conversion
table. Brinell and Vickers values below 300 are very close.)
The metal’s hardness indicates its relative response to the
forces exerted while working it. (Table 1.4)
When metals are hammered or rolled, they respond differently.
Malleability (literally meaning “hammer ability”)
refers to the capacity of a metal to be altered by such forces.
Gold is the most malleable metal, followed by silver and
aluminum. Gold can be rolled thinner without annealing
than can any other metal. In fact, gold can be rolled or
eaten so thin that light passes through it with a greenish
tint. The comparative malleability of metals in descending
Strength is the property of a metal to resist permanent
Tensile strength is a measurement of the maximum load
that can be applied to metal without the occurrence of
necking (localized reduction in diameter) or fracture.
Ultimate strength or UTS is the maximum stress a material
can withstand, the point at which any further stress will
result in necking and weakening.
When stress is applied to metal, it deforms. When the stress
is below a certain threshold the metal will return to its original
shape when the stress is removed. This is called elastic
deformation. The range of this temporary deformation is
called the elastic zone.
Plastic deformation is what happens when a metal is
deformed beyond its elastic deformation point. It is not possible
to accurately measure the exact transition between
elastic and plastic deformation. To provide a useable reference,
a permanent deformation of 0.2% was chosen to represent
the stress needed to cause plastic deformation.
Yield strength is the aspect of tensile strength that indicates
the amount of force or stress required to permanently
deform a metal by 0.2 percent.
Malleability indicates the ability of a metal to be formed
by compression (such as by being struck with a hammer)
Ductility refers to the ability of a metal to be elongated or
drawn into a fine wire without breaking. Again, gold is the
most ductile metal, permitting it to be drawn finer than any
chapter 1 | Precious Metals 11
other metal can without breaking. Second is silver, followed
by platinum. The comparative ductility of metals in
descending order is:
One measure of ductility is elongation to break, or the
length to which metal can be stretched before it will break,
expressed as a percentage.
Malleability is related to ductility but not all malleable
metals are ductile. Gold is both malleable and ductile;
lead is malleable but not ductile.
A sugar cube weighs less than a cube of gold the same size,
the reason being that gold is denser, or weighs more for the
same volume. Density is measured as weight per unit of
volume, or specific gravity. It is expressed as grams per
cubic centimeter (g/cm3) as compared with water, which
has a specific gravity of 1 g/cm3. Gold is very dense. With a
specific gravity of 19.32, its weight is almost twenty times
greater than the same volume of water. The density of gold
explains why prospectors find gold when panning. Because
of its high specific gravity (density) gold sinks to the bottom
of any stream. When comparing the relative cost of making
an item in 14k or 18k gold, one must consider that 18k will
weigh more for the same volume because of its higher specific
Melting point is defined as the point below which a metal
is solid and above which it is liquid. Pure metals have a
specific melting point, but most alloys have a temperature
range where they are neither completely solid nor completely
liquid (Table 1.5). When an alloy is heated, it
reaches a point at which it is no longer a solid but is not yet
fully liquid. This is called its solidus point.
12 Professional Jewelry Making
As the metal is heated further it reaches its liquidus point,
the point at which the metal is totally liquid. In this range
between solidus and liquidus, the metal has a slushy consistency.
Pure metals do not exhibit such a range.
The exceptions are alloys that transition from liquid to
solid at a specific melting point. These are called eutectic
alloys and can be defined as the mixture with the lowest
melting temperature alloy. Not all alloy systems have a
eutectic, but a very important one for jewelers is in the
silver-copper system where the eutectic alloy is 71.9%
silver and 28.1% copper with a melting point of 1435°F
(779°C). The presence of the silver/copper eutectic is felt
not only in sterling silver melting and solidification
behavior but also in silver solders and even in gold alloys
that contain a significant amount of silver and copper
such as 14k yellow with its relatively low melting point.
As an electric current passes through different materials,
it meets a resistance characteristic for that material. In
general, metals are good conductors of electricity. Silver
has the best electrical conductivity, because it presents
the least electrical resistance. Copper is the second best
electrical conductor with gold being third. This high
conductivity, combined with its superior resistance to
tarnishing, makes gold ideal for use in solid state circuitry
(Table 1.6). Like electricity, heat passes through materials
in differing ways. Silver is the best thermal-conductive
material, again with copper being second and gold the
third-best thermal conductor (Table 1.7).
Resistivity at 0ºC
Source: Grimwade 2009.
Table 1.6 electrical resistance of precious metals.
grAIn strUctUre And
Metals have a crystalline structure. These crystals, often
referred to as grains, change in size and orientation as a
result of external forces. Cold working precious metals
increases their hardness and decreases their malleability
and ductility. When metal is initially cast into an ingot
or into a finished piece of jewelry, the grain structure is
random, and the size of the grains is large. Such metal is
soft and workable (Illustration 1.2). When working metals,
the grains become packed together. Processes such as
bending, forming, rolling, and twisting compress the grains
and make the metal harder. The result, known as work
hardening, may be desirable for components that require
springiness or hardness, such as cuff bracelets, clasp
elements, pinstems, and hinge pins (Illustration 1.3).
With continued working, the metal becomes even harder
and more resistant to external forces because of the further
compaction of the grains into an elongated and flatter
configuration (Illustration 1.4). If the metal is pushed even
further, it will eventually break along the boundaries of the
grains. This phenomenon is exhibited when repeatedly
bending a wire coat hanger back and forth to break it. To
avoid overworking and consequent cracking, metal should
be annealed when its thickness has been reduced to
approximately 50 to 75 percent of the starting point. This
can be measured when rolling, drawing, or forging a piece
of metal but it is difficult to measure when bending,
forming, or twisting. For this reason, be sensitive to an
increase in hardness as a result of cold working.
0 to 100ºC
Source: Grimwade 2009.
Table 1.7 Thermal conductivity of precious metals.
Illustration 1.2 Grain structure of
fully annealed metal.
After a significant amount of cold work has hardened
metal, a workable state can be restored through a process
called annealing, which entails heating metal to an appropriate
temperature. During this process, the stretched
deformed grains recrystalize into larger sizes and more uniform
shapes, restoring a metal’s workability. Although it is
difficult to measure the temperature of a metal during this
process, the color of both the metal and the flame are indicators.
For maximum annealing and the corresponding
increase in workability, heat the metal to the proper temperature
(and color) (Table 1.8).
The effects of annealing are subject to both the variation in
duration and the temperature of heating. Short annealing
times and lower temperatures relieve residual stress in the
metal with virtually no change in the size of the grains,
Illustration 1.3 Grain structure of
partially work hardened metal.
whereas higher temperatures result in increased malleability
and ductility, decreased hardness, and larger grain size.
Overheating the metal will result in even larger grains that
are visible to the naked eye, accompanied by a decrease in
workability. It is important to anneal a piece of metal uniformly,
to avoid creating differential grain sizes and consequent
variations in hardness.
Although greater control during heating can be achieved
in a kiln, most jewelers anneal metal by heating it on a
charcoal block with a torch. Observe the color during heating
by placing the work in a darkened area. Use a broad
reducing flame over the entire object, or systematically
heat the metal in sections. Bundle wire tightly to avoid
accidental melting. During heating, watch the color to
determine when annealing has occurred. Other visual indications
of annealing are when flux becomes molten and
when the tip of a torch flame turns yellow-orange as it is
Approximate Annealing Temperatures
Metal ºC ºF Color by Eye
fine Gold 200 400 Black heat
fine Silver 200 400 Black heat
22k colored Golds 550 1000 Very dark red
18k colored Golds 550–600 1000–1100 Very dark red
14, 10, & 9k colored Golds 650* 1200 Dark red
Palladium White Golds 650–700 1200–1300 cherry red
Nickel White Golds 700–750** 1300–1400 cherry red
Sterling Silver 600–650 1100–1200 Dark red
Platinum 800 1500 Bright red
* colored golds of 18k and less should be water quenched from the annealing temperature to retain softness and ductility.
** Ni-white golds should be air-cooled to minimize phase separation and color change.
Source: adapted from Grimwade 2009.
Table 1.8 Typical annealing temperatures for precious metals and their alloys.
chapter 1 | Precious Metals 13
Illustration 1.4 Grain structure of
fully work hardened metal.
14 Professional Jewelry Making
played on the surface. After annealing, remove the flame or
cover the metal in a fuel-only (yellow) flame to reduce oxidation
in cases where oxidation is a problem. When the
metal has lost its reddish glow, quench it in water (except
for nickel white-gold alloys, which are air cooled). Immerse
the annealed metal in a warm pickle solution to remove
the surface oxides.
Slow cooling may result in effects similar to heat treating,
in which the metal is partially hardened by holding it at a
low temperature for an extended period. Many alloys can
be intentionally “heat treated” or “age hardened,” with
each alloy having its own time and temperature
A number of methods for measuring, or assaying, the quality
of precious metals have been used for centuries, particularly
to determine the gold content of gold-bearing alloys.
Fire assay, or cupellation, has been used for nearly 4500
years. It is an extremely accurate procedure in which scrapings
of an alloy are subjected to a series of elaborate steps
that include weighing, melting, rolling, dissolving in acid,
and reweighing. The beginning and ending weights are
compared to determine the fineness of the original sample.
The touchstone or acid testing procedure has also been in
use for centuries. This system is quick and simple but not
as accurate as fire assaying. In this method, the alloy in
question is rubbed on a smooth dark stone next to a similar
rubbing from a standard alloy of known content. A set
of test needles with tips ranging in purity is used as the
standard. A stripe of acid is spread across both rubbings,
and the results are compared. The rubbing with the higher
gold content will be more resistant to the acid and leave a
clearer, brighter stripe. Although this system is dependent
on visual comparison, it is sufficiently accurate for use in a
jewelry workshop. CAuTion: Acid is highly corrosive and
harmful if brought into contact with skin or eyes.
16 Professional Jewelry Making
Even though goldsmiths produce objects in precious
materials, this book stresses the value of the process
rather than the product. In other words, the real value
is to be found not in the finished ring or chain but in the
procedures by which it is created. Rings and chains may
wear out with time, but mastery of the techniques that make
beautiful objects is timeless.
Strive for perfection at every point. The first step in making
a piece of jewelry is always the most important, that is,
until the second step comes along. Just as the placement of
the four corners of a building determines the course of the
construction that follows, in making jewelry, layout is also a
critical step. The finished product will never be more accurate
than the first step.
Although the ultimate goal is to work both flawlessly and
rapidly, the novice should concentrate exclusively on the
former. Ordinarily, the first time a craftsman attempts a
new project it can take as much as three times longer than
the time required by an experienced craftsman. You cannot
cut corners until you know where they all are. Speed
comes with practice. As the project nears completion, look
for areas that need a little more attention. There will always
be some way to improve your work. Do not stop until you
are convinced that you have done the best job possible,
even if it takes longer than you expected. In the end, the
results will be worth the effort.
tHree stePs for correctIng
errors And ImProVIng
First, closely examine and analyze your work. Take measurements
with calipers, dividers, spring gauges, machinists
squares, and flat edges, to check angles, flatness, and
dimensions and to make comparisons. It is often helpful to
use a marker to write the measurements on the work itself.
During this step, concentrate on studying the situation; do
not even consider the remedy yet.
Next, try to figure out what is wrong and plan actions to
correct or improve it. Consider filing, sanding, sawing,
forging, or other techniques. Imagine the tools in your
hands and their effects on the metal. Do not begin working
until you have studied and planned, step by step, all facets
of your action. Finally, when you have thought it out and
you are absolutely sure what to do, take action and execute
Frequently when novices are confronted with the prospect
of making a simple yet tedious component for a piece of
jewelry, such as a jump ring or a piece of tubing, they ask
whether there isn’t an easier way, such as purchasing the
element commercially. It is often easier to purchase commercial
parts—in fact, it would be even easier to purchase
the entire piece of jewelry! But remember that it is the
mastery of technique that yields the greatest satisfaction.
Aside from pride in craftsmanship, there are several practical
reasons for developing the skill and knowledge to make
every component of your work. First, the design may call
for a finding in an uncommon size, color, karat, or shape
that cannot be purchased. Even if the finding you require
is available, deadlines often preclude waiting to receive it.
No matter how well trained and experienced a craftperson
is, there will always be new and unexpected challenges.
Goldsmiths are often asked to make items of jewelry that
are unlike anything they have encountered before. In cases
like these, craftspeople must improvise and seek new solutions
that may be a variation of techniques that they have
used previously. Sometimes they even must create new
techniques. In many ways, the test of a master is not what
he or she already knows but what he or she can improvise
based on similar experiences and the requirements of the
project at hand. With the pressures of a commitment pushing
from behind, necessity becomes the mother of invention.
Sometimes this will result in failure, but more often it
will result in success. In either case there is something
valuable to be learned.
UsIng tHe metrIc sYstem
The metric system originated in France around 1790.
Although the United States was the first country to introduce
metric currency—the dollar in 1789—it has been
one of the slowest to adopt the metric system of measurement.
Nonetheless, most countries in the world use only
the metric system of meters, liters, and grams. Calcula-
tions are far simpler in the decimal-based metric system
in which 1 meter equals 100 centimeters which equals
1000 millimeters, rather than the English system in
which 1 yard equals 3 feet and 1 foot equals 12 inches and
then inches are divided into either fractions or thousandths.
The basic metric unit used in jewelry is the millimeter,
which is far smaller than the inch of the English
system. For jewelry work, the metric system is superior to
the English system because it is more precise and far easier
Goldsmithing demands attention to minute details. The
very nature of fabricating small objects with hinges, clasps,
settings, and so on requires that the components fit
together well. The tolerance for jewelry handwork in this
book is one-tenth of a millimeter, 0.1 mm, which is only
about twice the diameter of the average human hair. That
means that every piece of metal should be measured and
corrected so that its dimensions are within 0.1 mm of the
given specifications. Sometimes a greater error will be
hardly noticeable, but in most cases, a variation of more
than 0.1 mm will cause problems with fit or function.
Accordingly, it is important to have accurate measuring
tools at hand, several of which are described in Chapter 3.
Although I have made every effort to give accurate specifications
for the projects in this book, in reality some variation
is understandable owing to the nature of handwork. Be
sure to keep in mind, however, that the closer the components
are to specification, the easier will be the job of fitting
Illustration 2.1 combination metric and english ruler (shown at 100 percent).
chapter 2 | General Procedures 17
It has been said that “nothing else feels like gold.” And
although there is nothing quite like working in real karat
golds, in fact most techniques can be applied to nonprecious
metals. Nickel alloys, brass, and copper all saw,
file, bend, solder, anneal, forge, form, and roll in nearly
the same way as gold and silver. The benefits of learning
with nonprecious materials outweigh the very small
advantage of working in gold, silver, or platinum. As an
analogy, the difference between driving a car at 40 or 60
requires no conscious adjustment; adapting what you do
comes naturally once you know how to drive. Similarly,
although the melting temperature of gold solder is
higher than that of the silver solder you will use on brass
or copper, the process of soldering is the same and
adjustment to differences such as these will quickly
An item made of precious metals is likely to be worn, given
away, or sold, whereas an item created out of materials
without intrinsic value will be saved for future reference.
Imagine trying to replicate a project—or even worse, trying
to make a variant of a project you made ten years earlier—
without the benefit of holding the original in your hand.
But if you have saved the original sample as a reference
along with good notes, you can easily reproduce the process
and replicate or alter the product to suit your current
needs. A collection of nonprecious samples also serves as a
three-dimensional portfolio, demonstrating the skill of the
maker to potential employers and customers. Such a collection
is small, portable, and durable, and it speaks for
itself. While nonprecious samples have no intrinsic value,
in actuality they are worth more than their weight in gold.
18 Professional Jewelry Making
Torches produce heat by sustaining combustion while
feeding two different gases into the flame. In oxygen-fuel
torches, both gases are supplied under regulated pressure:
oxygen from a pressurized tank, combined with fuel from
either a tank or city-gas supplied to the building. In air-fuel
torches, fuel from a tank combines with air drawn either
from the atmosphere, or supplied by a pressurized tank.
Three different types of flames are important to goldsmithing.
A cool reducing flame has a pale blue flame with a yellowish
tip, because there is more fuel than oxygen. A soft,
bushy reducing flame is ideal for annealing and melting.
Because of its size and composition, such a flame shields
the surface from atmospheric gasses while absorbing oxygen
that might otherwise combine with the metal.
With the addition of more oxygen, a neutral flame is
achieved. Such a flame is all blue, without any yellow at
the tip. This flame has a softly defined bright blue inner
cone within a pale blue outer cone. This type of flame is
ideal for most soldering jobs where a large area can safely
be heated. The hottest point of the flame is the tip of the
When even more oxygen is added to the flame, the inner
blue cone becomes smaller, sharper, and brighter. An oxidizing
flame such as this emits a hissing sound as excess
oxygen is forced into the flame. Useful for delicate soldering
jobs where the heat must be intense and localized, this
type of flame floods the work with unconsumed oxygen
which can result in oxidation (tarnish). If used when melting,
this flame will damage the metal.
There is no need to buff and polish work that is executed as
a learning exercise. In fact, in some countries, candidates
taking the practical portion of the test for their goldsmiths
and master goldsmiths credentials are not permitted to polish,
electroplate, engrave, or set stones into their work. The
reason is that polishing hides the craftsmanship by diminishing
sharp corners and crisp surfaces. By leaving a finely
sanded (satin) finish, therefore, the craftsmanship is
revealed for examination.
This said, we should also note that the appeal of jewelry
depends largely on its finish. Polishing is the most common
finish for jewelry made of precious metals, because it
exploits their unique reflectivity and lustre. Buffing and
polishing are a specialty apart from goldsmithing. Although
basic techniques do not require much experience, more
sophisticated techniques do call for a vast range of expertise
and equipment. Because the focus of this book is on goldsmithing,
we shall only briefly touch on buffing and
In general, jewelry made of precious metals should be
sanded to a fine finish in preparation for polishing. A piece is
usually sanded to remove filing marks, scratches, and imperfections
after all other work such as soldering, hammering,
and filing have been completed. Sometimes, however, a
complex piece with several components is sanded and
polished before it is assembled because afterward some of
the components will be inaccessible for polishing. During
or after a piece is completed, sanding progresses from coarse
abrasive paper (220-grit) to finer grades (400-600-grit),
changing direction with each step up in fineness. A general
guideline is that large flat surfaces (which are difficult to
polish) should be sanded to a higher prepolish finish with
fine (600-grit) paper. Sanding sticks and sanding drums are
good for holding abrasive paper and cloth. Other commercial
and custom-made wheels and jigs can be used for sanding.
Before going on to buffing, check to make sure that all
of the file marks and scratches have been removed.
The responsibility of the goldsmith ends when the construc-
tion and finishing of a piece of jewelry are complete. If an
item has stones to be set, this usually will be done by a stone
setter, an artisan with specialized training and skills.
Although contemporary jewelers frequently set their own
stones, stone setting is a field encompassing complex techniques,
that are too numerous to be included in this book.
The following are a few general suggestions regarding the
projects in this book and goldsmithing as a whole:
• Keep your work clean as you proceed. Use an abrasive
pad to remove grease and oxides and to impart a fine satin
finish during fabrication. It is easier both to see and to
work on clean components.
• With most projects it is best to work from the inside out.
That is, always file, sand, and polish the inside of rings
(and most other items) first.
• A basic rule in goldsmithing is to work up a shape evenly
and uniformly. If several components or parts of components
are to match, bring them all up to form at the
same time. Rather than concentrating on one area until
it is finished, work alternately on all areas, collectively
bringing the entire piece to the same stage of
• Carry each step to the limit of your ability. Take a short
break and then return to the work, looking for ways to
improve the results even further.
• As you read through this book, remember that there is
usually more than one way to do most jobs. Knowing
only one tool or technique for a particular job, will not
be enough because the method that usually works may
not solve a slightly different problem. Be open to suggestion.
Never discard someone else’s method, but file it in
the back of your mind for the time when your old way
will not work.
chapter 2 | General Procedures 19
Although the procedures in this book are performed safely
by thousands of goldsmiths every day, newcomers and
experienced jewelers alike need to observe some safety precautions.
Above all, concentrate on what you are doing
whenever you are working with hazardous materials or
tools. Consider what could happen and prevent accidents.
Accidents take only a second to occur, so do not allow
yourself to be distracted—even for a second. Note particularly
• Acids can be extremely dangerous, so do not let them
touch your skin and do not inhale the fumes. Contact
with eyes can be especially harmful; for this reason wear
a full face shield when working with acids and chemicals.
Some workers wear safety glasses whenever they are
in the studio. Pickling solution is kept warm and so
should be used with adequate ventilation. Keep an open
box of baking soda near the pickle pot for the immediate
neutralization of acid spills. Quench metal in water or
air cool it before submerging it in hot pickling solution.
Never throw metal into the pickle; instead, use copper
tongs to slide it into the solution without splashing.
• Torches and melting equipment are inherently hazardous,
so never use them recklessly or even casually.
• Spinning tools such as a flex shaft, polishing lathe, and
bench grinder can eject small particles at high velocities.
Always wear goggles, tie back long hair and sleeves, and
keep your fingers clear of the spinning tool. In addition,
when polishing, do not entrap your fingers in work that
could be grabbed by such rotating tools.
• Sharp tools such as files, drills, and gravers can cause injury
and should be handled with care. Consider the effects
of slipping with a sharp tool, and position your fingers
• Fumes can be hazardous if inhaled. They are emitted by
the pickle bath, solvents, glues, solders, and by drying
correction fluid (used as an antiflux). Work in well-ventilated
areas and avoid inhaling fumes.
20 Professional Jewelry Making
We should explain here our protocol for the usage of safety
alerts throughout the book.
Acid can be extremely dangerous. Avoid direct contact with
the skin. Do not inhale the fumes. Contact with the eyes can
be very harmful and for this reason a full face shield is
advised when working with acids.
Pickle: Pickling solution is kept warm and should be used
with adequate overhead ventilation. Keep an open box of
baking soda near the pickle pot for immediate neutralization
of acid spills. Metal is quenched in water or air cooled
prior to submersion in hot pickling solution. Never throw
metal into the pickle. Instead, use copper tongs to slide it
into the solution without splashing. Think carefully before
putting hot metal into hot pickle, because this is hazardous
and forces the pickle into areas where it will be difficult to
remove later. Do it only with extra face and hand protection
and great caution. The submersion of hot metal into hot
pickle increases the effects of pickling, resulting in acid
leeching (depletion plating).
Follow proper fire safety procedures, observe all gas handling
rules, and use proper ventillation. Keep all flammable
items away from the soldering area. Wear fire-resistant
clothing and shoes. Tie back long hair and sleeves. Refer to
the pickling safety procedures for cleaning metal after
Dopping Wax, Shellac, and Jett Sett: Dopping wax
and shellac, used to hold metal pieces when working, are
melted with a cool, yellow (fuel-only) flame. Do not drip
hot wax onto your skin. Do not overheat the wax. If it
smokes, it is too hot. Avoid inhaling fumes from melting or
smoking wax. Dopping wax dissolves in acetone, which is
toxic. Shellac is a safer alternative because it dissolves in
alcohol. Avoid breathing solvent fumes. Jett Sett is one
brand of a plastic that becomes malleable in hot water and
is used as an alternative to dopping wax and shellac in
many applications. No solvents are required.
Soldering: Avoid solders containing cadmium or antimony.
Avoid fluxes containing flouride. Avoid skin contact
with boric acid and do not ingest.
Soldering Hollow Forms: Drill a small vent hole before
soldering a hollow form to allow expanding gasses to
escape safely. The hole allows gas to move in and out during
heating and prevents explosion.
Soldering a volumetric form closed is difficult and even
hazardous. The problem is that air gets trapped and then
expands tremendously when heated, especially if it contains
any moisture. The expansion of the internal gas makes it
difficult to solder a form completely closed. The force of
the expanding gas may even blow a hole in the piece with
the force of a firecracker, sending hot metal flying across
Soldering Platinum: Because of the high melting
temperature of platinum and platinum solders, use at least
#5 filtered soldering/welding goggles when welding and
soldering platinum. Annealing, soldering or welding
platinum without filtered eye protection could lead to
serious eye damage. Do not remove your glasses until the
glow dissipates from the piece. Because of the high heat
involved in annealing and soldering platinum, be sure the
piece is completely quenched or air cooled before handling
it. A plastic or glass quench bowl is not recommended.
Antiflux: Antiflux is a fluid that can be painted on seams
before soldering to prevent solder from flowing again. If
using typwriter correction fluid as an antiflux, paint it on
seams and let it dry. Do not inhale the fumes and use proper
ventillation during application and soldering.
Investment contains silica and is dangerous if inhaled. Use
with proper ventillation and wear a dust mask. Avoid skin
and eye contact. Investment removal should be performed
under a fume hood or with appropriate protection.